High crystalline quality ZnBeSe grown by molecular beam epitaxy with Be}Zn co-irradiation
Journal of Crystal Growth 208 (2000) 205}210 High crystalline quality ZnBeSe grown by molecular beam epitaxy with Be}Zn co-irradiation S.P. Guo , Y. Luo , W. Lin , O. Maksimov , M.C. Tamargo *, I. Kuskovsky , C. Tian , G.F. Neumark Center for Advanced Technology on Photonic Materials and Applications, Center for Analysis of Structures and Interfaces (CASI), Department of Chemistry, City College-CUNY, New York, NY 10031, USA School of Mines and Department of Applied Physics, Columbia University, New York, NY 10027, USA Received 4 June 1999; accepted 6 July 1999 Communicated by A.Y. ChoAbstract High crystalline quality ZnBeSe epilayers with di!erent compositions were grown on GaAs substrates by molecularbeam epitaxy using Be}Zn co-irradiation of the III}V surface and a ZnSe bu!er layer. A (1;2) re#ection high-energyelectron di!raction pattern was formed after the Be}Zn co-irradiation indicating the formation of Be and Zn dimers onthe GaAs surface. A two-dimensional growth mode was observed throughout the growth of the ZnSe bu!er layer andZnBeSe epilayer. Narrow X-ray linewidth as low as 23 arcsec with the etch pit density of mid 10 cm were obtained.The linewidth of the dominant excitonic emission is about 2.5 meV at 13 K for the near-lattice-matched ZnBeSe layer.For a nitrogen-doped sample, capacitance}voltage measurements showed a net acceptor concentration of2.0;10 cm. In addition, the use of a BeTe bu!er layer and of a Zn-irradiation with a ZnSe bu!er layer were alsoinvestigated. 2000 Elsevier Science B.V. All rights reserved.PACS: 81.15.Hi; 80.05.Dz; 78.55.Et; 61.10.EqKeywords: Molecular beam epitaxy; ZnBeSe; Irradiation; X-ray di!raction; Photoluminescence1. Introduction onstrated for the rst time in 1991 [1,2]. By intro- ducing a ZnMgSSe quaternary alloy and ZnSSe Recently, there is much interest in developing ternary alloy lattice matched to the GaAs substrateblue}green laser diodes (LD) and light-emitting as the cladding layer and waveguiding layer anddiodes. Blue}green LD based on ZnSe were dem- strained ZnCdSe as the active layer, blue}green LD under continuous-wave operation with lifetimes of about 400 h have been achieved . However, dur- ing molecular beam epitaxial (MBE) growth, the * Corresponding author. Tel.: #1-212-650-6147; fax: #1-212-650-6848. sulfur sticking coe$cient depends strongly on the E-mail address: email@example.com (M.C. Tam- substrate temperature, making it extremely di$cultargo) to avoid composition #uctuations in the ZnMgSSe0022-0248/00/$ - see front matter 2000 Elsevier Science B.V. All rights reserved.PII: S 0 0 2 2 - 0 2 4 8 ( 9 9 ) 0 0 4 2 4 - 8
206 S.P. Guo et al. / Journal of Crystal Growth 208 (2000) 205}210alloys . With a small lattice constant (5.139 A)s In this letter, high crystalline quality ZnBeSeand a large band gap (E 5 eV), BeSe is a very epilayers were achieved by using Be}Zn co-irradia-good candidate to replace ZnS in the quaternary tion before the ZnSe bu!er layer growth. A (1;2)and ternary alloys. It is also important to note that surface reconstruction was observed on theMBE growth is much more controllable and repro- (0 0 1)GaAs surface after the co-irradiation indicat-ducible when an alloy contains several metals and ing the formation of a Be and Zn surface termina-only a single nonmetal, rather than several non- tion layer. A two-dimensional growth mode wasmetals. In addition, Beryllium chalcogenides have obtained immediately on this surface upon initia-a high degree of covalent bonding compared to tion of the ZnSe layer. In situ re#ection high-energyother wide gap II}VI semiconductors and are ex- electron di!raction (RHEED) and ex situ X-raypected to have higher bonding energies , which di!raction (XRD), EPD and photoluminescencemay further improve the device lifetime. However, (PL) were used to characterize the crystalline qual-in growth of II}VI alloys on III}V substrates con- ity. p-Type doping of ZnBeSe by nitrogen was alsotrol of the II}VI/III}V interface can be a problem. performed. The doping level was determined byWe have found that the quality of the interface is capacitance}voltage (C}) and electrochemicalappreciably improved by performing a Zn}Be C} (ECV) measurements.co-irradiation of the III}V surface. The II}VI/III}V interface quality is extremelyimportant for the growth of II}VI materials on 2. ExperimentIII}V substrates. Improvement of the II}VI/III}Vinterface has been the main reason for the reduction ZnBeSe epilayers were grown on (0 0 1)GaAsof the defect density obtained in the past. In the substrates in a Riber 2300 MBE system withcase of the growth of ZnSe-based materials on a III}V chamber and a II}VI chamber connectedGaAs, it is important to avoid any tendency to by ultra-high vacuum. Oxide desorption of the sub-form a Se-(2;1) surface reconstruction  on the strate was performed in the III}V chamber by heat-GaAs surface. On such a surface, isolated islands ing to 5803C under an As #ux, after whichare easily formed, and very high density of stacking a 300 nm GaAs bu!er layer was grown. The mainfaults are produced believed to be related to the shutter was closed at a substrate temperature (¹ ) formation of Ga Se at the interface. By using of 5503C to maintain a (2;4) RHEED pattern. In Zn-irradiation to avoid the formation of Ga Se , order to avoid the formation of Ga Se at the a reduction of etch pit density (EPD) in the III}V/II}VI interface we performed Be}Zn co-ir-ZnSe/GaAs system from 10 to 10 cm has been radiation before the growth of 5 nm ZnSe bu!erreported . layer. Once the substrate with the GaAs bu!er With a few monolayers (ML) of ZnSe bu!er layer layer was transferred in vacuum to the II}VI cham-directly grown on the GaAs substrate, ZnBeSe epi- ber, the main shutter was opened immediately withlayers with X-ray linewidth of 27 arcsec have been the Zn and Be shutters open for 20 s. The RHEEDdemonstrated by Bousquet et al. . The EPD in pattern changes from (2;4) to (1;2) after thethe ZnBeSe layers are high in the 10 cm range, Be}Zn co-irradiation, indicating the formation ofwhich is much higher than that reported in the a new surface reconstruction on the (0 0 1)GaAsZnSe/GaAs system. By using a few ML of BeTe as surface. Then the ¹ was increased to 2503C and a bu!er layer, ZnBeMgSe with X-ray linewidths the ZnSe bu!er layer was grown. The RHEEDdown to 20 arcsec and EPD below 5000 cm pattern remains streaky and the surface reconstruc-was reported by Fischer et al. . However, due to tion changes from (1;2) to (2;1) during the ZnSethe high conduction band o!set of about 2.3 eV growth. After this the ¹ was increased to 2703C between BeTe and GaAs as well as between BeTe and 1 m-ZnBeSe epilayer was grown underand ZnSe the BeTe bu!er may produce a very high Se-rich conditions using elemental Zn, Be and Sepotential barrier for electrons, possibly a!ecting Knudsen e!usion cells. The RHEED pattern re-device performance. mains streaky (2;1) during the ZnBeSe growth.
S.P. Guo et al. / Journal of Crystal Growth 208 (2000) 205}210 207The p-type doping was achieved by employing an ments were performed at 13 K using the 325 nmOxford RF nitrogen plasma source. Two other line of the He}Cd laser for excitation. C}approaches to control the II}VI/III}V interface measurements were carried out at room temper-were also pursued. In one, a Zn irradiation with ature using a gold contact with a diameter ofa ZnSe bu!er layer was used. Once the substrate 0.6 mm.with the bu!er layer was transferred to the II}VIchamber, the substrate was heated to 2503C. When¹ was stable, the main shutter was opened with 3. Results and discussion the Zn shutter open for 20}60 s. Then the Se shutterwas opened to start the growth of the 5 nm of ZnSe. The full-width at half-maximum (FWHM) of theThe RHEED pattern is streaky (2;1) with super- double-crystal X-ray rocking curves (DCXRC) ofimposed weak elongated spots evident after the ZnBeSe epilayers grown under the three growthZnSe growth. After this the ¹ was increased to conditions described is shown in Table 1. The re- 2703C and ZnBeSe was grown. The RHEED pat- sults indicate that the crystalline quality of ZnBeSetern becomes streaky (2;1) gradually as growth was dramatically improved by using either a Be}Znproceeds. In the second, a BeTe bu!er layer was co-irradiation with a ZnSe bu!er layer or a BeTeused. Here, once the substrate with the bu!er layer bu!er layer. Fig. 1 shows the (0 0 4) re#ectionwas transferred to the II}VI chamber, the substrate DCXRC for a ZnBeSe epilayer with 3.1% Bewas heated to 3503C and a few ML of BeTe were grown with Be}Zn co-irradiation. A narrow peakdeposited under Te-rich conditions. The BeTe buf- related to the ZnBeSe epilayer, with a FWHM of 23fer layer was grown at 3503C instead of 2503C in arcsec was observed indicating very high crystallineorder to improve BeTe crystalline quality . The quality. From the (1 1 5) a and b asymmetricalRHEED pattern is streaky (2;1) after the BeTe re#ection DCXRC we can obtain the perpendiculargrowth. Then the ¹ was decreased to 2703C and and parallel lattice constants: a and a . The bulk ZnBeSe was grown. The RHEED remains streaky lattice constant then is calculated from the equa-(2;1) during the ZnBeSe growth. tion The ZnBeSe crystalline quality and Be composi- aa +1![2 /(1# )][(a !a )/a ],.tion were assessed by single and double crystal XRD measurements using a double-crystal biaxial Here is the Poissons ratio (we use the value ofdi!ractometer and Cu K radiation. For EPD for ZnSe of 0.28 for the ZnBeSe because of the measurements, a solution of methanol with 0.2% Br small Be composition). Assuming that Vegards lawwas used at RT, which has been demonstrated to be is valid for ZnBeSe, the Be composition can besuitable for ZnSe . A solution of concentrated assessed from the lattice constant. The dependenceHCl (32%) was also used at 603C, which has been of Be composition on Be cell temperature was in-reported to be a suitable etchant for quaternary vestigated for compositions near the lattice-match-ZnMgSSe  and ZnBeMgSe . PL measure- ed regime. The data are plotted in Fig. 2. A nearTable 1Properties of ZnBeSe epilayersGrowth conditions FWHM of DCXRC EPD (cm) FWHM of PL 13 K (arcsec) (meV)Zn-irradiation and ZnSe bu!er layer 300 10 5Be}Zn co-irradiation and ZnSe bu!er 23}45 Mid 10 2.5layerBeTe bu!er layer 18}40 Low and mid 10 2.5
208 S.P. Guo et al. / Journal of Crystal Growth 208 (2000) 205}210Fig. 1. (0 0 4) re#ection DCXRC for an undoped Zn - Fig. 2. Dependence of Be composition of Zn Be Se alloys on V VBe Se layer grown after Be}Zn co-irradiation of the GaAs the Be cell temperature during growth. Squares were calculated from the (1 1 5) a and b re#ection DCXRC, and the circle wassurface. The solid line is the experimental data and the dottedline is the Gaussian t. calculated from the (0 0 4) re#ection single crystal XRD data assuming that the epilayer is completely relaxed.linear dependence was observed within the small our system since we use a normal Se K-cell and wecell temperature range investigated, from 923 to did not perform a growth break.9603C, indicating a high level of compositional Fig. 3 shows the 13 K PL spectra for undopedcontrol in the growth of this alloy. ZnBeSe epilayers grown using (a) Be}Zn co-ir- The results of the EPD measurements are also radiation with a ZnSe bu!er, (b) a BeTe bu!er andshown in Table 1. The EPD for the ZnBeSe epi- (c) Zn irradiation with a ZnSe bu!er. The spectrumlayers grown with Zn irradiation is very high for the Be}Zn co-irradiation (case a) is quite similar(10 cm), whereas that grown with Be}Zn co- to that for the BeTe bu!er layer (case b): veryirradiation or with a BeTe bu!er layer is much similar emission peaks near the band gap edgelower, in the 10 cm range. The quality of the (FWHM is +2.5 meV * Table 1) and negligibleRHEED pattern for the di!erent growth conditions deep level PL are observed. However, the spectrumused suggests that the high EPD for the Zn-irradia- for the sample grown with Zn irradiation (case c)tion case may be related to a rough growth front of shows a broad deep level emission at 2.55 eV,the ZnSe bu!er while the lower EPD for Be}Zn and the FWHM of the band edge peak is +5 meVco-irradiation and BeTe bu!er layer cases is related (Table 1). The inset of Fig. 3 is the semi-log plot ofto the formation of a very #at Be-based interfacial the PL spectrum near the band gap region for thelayer. Comparing the best EPD ((5000 cm) re- sample grown with Be}Zn co-irradiation (case a)ported in Ref.  (grown under a reduced Se back- (ZnBeSe with 3.1% Be). Several sharp emissionground: 1 h growth break with Se valved cracker lines can be observed. The transitions at 2.894 andclosed, Zn #ux on and cleaned shutters), the slightly 2.904 eV are assumed to be related to free excitonichigher EPD in our ZnBeSe epilayers grown under recombination. These are consistent with the re-both Be}Zn co-irradiation and/or BeTe bu!er ported values of free excitonic recombination inlayer may be due to the higher Se background in ZnBeSe with 2.8% Be . The dominant peak at
S.P. Guo et al. / Journal of Crystal Growth 208 (2000) 205}210 209 (1;2) surface reconstruction may play a major role in improving the ZnBeSe quality. It has been shown that the Se-rich (2;1) surface recon- struction originates from the formation of a full monolayer of Se dimers . A (1;2) surface recon- struction has been proposed to be related to Zn dimers  on the (0 0 1)GaAs surface. However, such a (1;2) surface reconstruction has never been observed before, even after Zn irradiation of the GaAs is performed. We attribute the (1;2) surface reconstruction in our case to the formation of a full monolayer of Be and Zn dimers. Further investiga- tions, such as scanning tunneling microscopy stud- ies should be performed to conrm this assignment. The well-ordered Be}Zn layer on the GaAs surface avoids the formation of Ga Se , decreasing stack- ing faults and improving the crystalline quality dramatically. The observation of the RHEED pat- tern also indicates that a two-dimensional growth mode is achieved immediately and persists throughout the growth of the ZnSe bu!er layer and ZnBeSe epilayer on this (1;2) surface reconstruc- tion. Therefore, the growth front is quite #at andFig. 3. Low-temperature (13 K) PL spectra for undoped only the presence of a few atomic steps can induceZnBeSe layers grown using (a) Be}Zn co-irradiation with a ZnSe the formation of lattice defects such as dislocations.bu!er, (b) a BeTe bu!er and (c) Zn-irradiation with a ZnSebu!er. The inset is the semi-log plot near the band gap region of In addition, due to the high degree of covalentspectrum (a). bonding in beryllium chalcogenides the formation energy for a stacking fault is high at the II}VI/ III}V interface and a lower density of stacking2.856 eV is then tentatively attributed to a deep faults is expected in this Be-containing alloy.bound excitonic recombination. The peaks at 2.828and 2.796 eV may be phonon replicas of this domi-nant transition. The highly resolved PL spectrum 4. Conclusionsobserved supports the assessment of very highcrystalline quality of this sample. We have investigated the MBE growth and Capacitance}voltage measurements were per- properties of ZnBeSe epilayers with di!erent Beformed on a N-doped Zn Be Se epilayer. compositions grown on GaAs substrates by using From the slope of 1/C versus a net acceptor a new method for II}VI/III}V interface formationconcentration (n !n ) of 2.0;10 cm was ob- involving a Be}Zn co-irradiation with a ZnSe buf-tained, which is comparable to the value obtained fer layer. A (1;2) RHEED pattern was observedby ECV measurements (1.6;10 cm). This re- on the (0 0 1)GaAs surface after the Be}Zn co-sult is similar to reported doping levels [8,13]. The irradiation, suggesting the formation of a fullPL results of this sample will be reported separate- monolayer of Be and Zn dimers. A two-dimen-ly. sional growth mode was achieved throughout the The reasons for the quality improvement of Be- ZnSe bu!er layer and ZnBeSe epilayer growth.based materials by using a BeTe bu!er layer have Narrow X-ray linewidths down to 23 arcsec withbeen discussed in Ref. . In the case of Be}Zn a very low etch pit density, of mid 10 cm, wereco-irradiation performed here, the formation of the obtained. The linewidth of the dominant excitonic
210 S.P. Guo et al. / Journal of Crystal Growth 208 (2000) 205}210emission is about 2.5 meV at 13 K for a near lat-  H. Heon, J. Ding, W. Patterson, A.V. Nurmikko, W. Xie,tice-matched ZnBeSe layer. For a nitrogen-doped D.C. Grillo, M. Kobayashi, R.L. Gunshor, Appl. Phys.sample, a net acceptor concentration of 2.0; Lett. 59 (1991) 3619.  E. Kato, H. Noguchi, M. Nagai, H. Okuyama, S. Kijima,10 cm was obtained by C} measurements. A. Ishibashi, Electron. Lett. 34 (1998) 282.ZnBeSe grown with the BeTe bu!er layer shows  D.C. Grillo, M.D. Ringle, G.C. Hua, J. Han, R.L. Gunshor,the similar crystalline quality to that grown under J. Vac. Sci. Technol. B 13 (1995) 720.Be}Zn co-irradiation with a ZnSe bu!er, where-  F. Fischer, Th. Litz, H.J. Lugauer, U. Zehnder, Th. Ger-as that grown under Zn-irradiation alone, with hard, W. Ossau, A. Waag, G. Landwehr, J. Crystal Growth 175/176 (1997) 619.a ZnSe bu!er has a much poorer quality.  D. Li, M.D. Pashley, J. Vac. Sci. Technol. B 12 (1994) 2547.  C.C. Chu, T.B. Ng, J. Han, G.C. Hua, R.L. Gunshor, E. Ho, E.L. Warlick, L.A. Kolodziejski, A.V. Nurmikko,Acknowledgements Appl. Phys. Lett. 69 (1996) 602.  V. Bousquet, E. Tournie, M. Laugt, P. Vennegues, J.P. H K H ` The authors acknowledge the support of the Na- Faurie, Appl. Phys. Lett. 70 (1997) 3564.  F. Fischer, M. Keller, T. Gerhard, T. Behr, T. Litz, H.J.tional Science Foundation under grant number Lugauer, M. Keim, G. Reuscher, T. Baron, A. Waag, G.DMR9805760. This publication was developed un- Landwehr, J. Appl. Phys. 84 (1998) 1650.der the auspices of the City University of New York  E. Tournie, V. Bousquet, J.P. Faurie, Appl. Phys. Lett. 72 HCAT in Ultrafast Photonic Materials and Applica- (1998) 2859.tions supported by the New York State Science and  A. Kamata, H. Mitsuhashi, J. Crystal Growth 142 (1994) 31.Technology Foundation.  M. Shiraishi, S. Tomiya, S. Tanigachi, K. Nakano, A. Ishibashi, M. Ikeda, Phys. Stat. Sol. (a) 152 (1995) 377.  H.J. Lugauer, Th. Litz, F. Fischer, A. Waag, T. Gerhard,References U. Zehnder, W. Ossau, G. Landwehr, J. Crystal Growth 175/176 (1997) 619. M.A. Haase, J. Qiu, J.M. dePuydt, H. Cheng, Appl. Phys.  A. GarcmH a, J.E. Northrup, J. Vac. Sci. Technol. B 12 (1994) Lett. 59 (1991) 1272. 2678.